LMucko/crystallography-open-database huggingface dataset:
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2373 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006776
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2373 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.352
_cell_length_b                   4.352
_cell_length_c                   4.352
_cell_formula_units_Z            4
_cell_volume                     82.426
_database_code_amcsd             0008358
_diffrn_ambient_temperature      2373
_exptl_crystal_density_diffrn    3.248
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006776
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2473 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006777
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2473 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.358
_cell_length_b                   4.358
_cell_length_c                   4.358
_cell_formula_units_Z            4
_cell_volume                     82.768
_database_code_amcsd             0008359
_diffrn_ambient_temperature      2473
_exptl_crystal_density_diffrn    3.234
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006777
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2573 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006778
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2573 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.371
_cell_length_b                   4.371
_cell_length_c                   4.371
_cell_formula_units_Z            4
_cell_volume                     83.511
_database_code_amcsd             0008360
_diffrn_ambient_temperature      2573
_exptl_crystal_density_diffrn    3.206
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006778
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2673 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006779
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2673 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.381
_cell_length_b                   4.381
_cell_length_c                   4.381
_cell_formula_units_Z            4
_cell_volume                     84.085
_database_code_amcsd             0008361
_diffrn_ambient_temperature      2673
_exptl_crystal_density_diffrn    3.184
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006779
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2773 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006780
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2773 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.396
_cell_length_b                   4.396
_cell_length_c                   4.396
_cell_formula_units_Z            4
_cell_volume                     84.952
_database_code_amcsd             0008362
_diffrn_ambient_temperature      2773
_exptl_crystal_density_diffrn    3.151
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006780
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2873 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006781
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2873 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.403
_cell_length_b                   4.403
_cell_length_c                   4.403
_cell_formula_units_Z            4
_cell_volume                     85.358
_database_code_amcsd             0008363
_diffrn_ambient_temperature      2873
_exptl_crystal_density_diffrn    3.136
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006781
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2973 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006782
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2973 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.408
_cell_length_b                   4.408
_cell_length_c                   4.408
_cell_formula_units_Z            4
_cell_volume                     85.649
_database_code_amcsd             0008364
_diffrn_ambient_temperature      2973
_exptl_crystal_density_diffrn    3.126
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006782
Cation ordering in NiAl2O4 spinel by a 111 systematic row CBED technique Sample: picrochromite
Tabira, Y.; Withers, R. L.; Physics and Chemistry of Minerals 27 (1999) 112–118; doi:10.1007/s002690050247

data_9006783
_publ_section_title
;
 Cation ordering in NiAl2O4 spinel by a 111 systematic row CBED technique
 Sample: picrochromite
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              112
_journal_page_last               118
_journal_paper_doi               10.1007/s002690050247
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Cr2 Mg O4'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.3327
_cell_length_b                   8.3327
_cell_length_c                   8.3327
_cell_volume                     578.572
_database_code_amcsd             0008365
_exptl_crystal_density_diffrn    4.415
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Cr2) O4'
_cod_database_code               9006783
Effect of pressure on the thermal expansion of MgO up to 8.2 GPa Sample: Run1 at T = 300 K, P = 0.00 GPa, measured at beginning of the experiments
Zhang, J.; Physics and Chemistry of Minerals 27 (2000) 145–148; doi:10.1007/s002690050001

data_9006784
_publ_section_title
;Effect of pressure on the thermal expansion of MgO up to 8.2 GPa Sample: Run1
 at T = 300 K, P = 0.00 GPa, measured at beginning of the experiments
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              145
_journal_page_last               148
_journal_paper_doi               10.1007/s002690050001
_journal_volume                  27
_journal_year                    2000
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.2131
_cell_length_b                   4.2131
_cell_length_c                   4.2131
_cell_volume                     74.783
_database_code_amcsd             0008366
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      300
_cell_formula_units_Z            4
_exptl_crystal_density_diffrn    3.580
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006784
Effect of pressure on the thermal expansion of MgO up to 8.2 GPa Sample: Run1 at T = 300 K, P = 0.00 GPa, measured at the end of the experiments
Zhang, J.; Physics and Chemistry of Minerals 27 (2000) 145–148; doi:10.1007/s002690050001

data_9006785
_publ_section_title
;Effect of pressure on the thermal expansion of MgO up to 8.2 GPa Sample: Run1
 at T = 300 K, P = 0.00 GPa, measured at the end of the experiments
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              145
_journal_page_last               148
_journal_paper_doi               10.1007/s002690050001
_journal_volume                  27
_journal_year                    2000
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.2136
_cell_length_b                   4.2136
_cell_length_c                   4.2136
_cell_volume                     74.810
_database_code_amcsd             0008367
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      300
_cell_formula_units_Z            4
_exptl_crystal_density_diffrn    3.579
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006785
Effect of pressure on the thermal expansion of MgO up to 8.2 GPa Sample: Run1 at T = 300 K, P = 2.65 GPa
Zhang, J.; Physics and Chemistry of Minerals 27 (2000) 145–148; doi:10.1007/s002690050001

data_9006786
_publ_section_title
;
 Effect of pressure on the thermal expansion of MgO up to 8.2 GPa
 Sample: Run1 at T = 300 K, P = 2.65 GPa
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              145
_journal_page_last               148
_journal_paper_doi               10.1007/s002690050001
_journal_volume                  27
_journal_year                    2000
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.1899
_cell_length_b                   4.1899
_cell_length_c                   4.1899
_cell_volume                     73.555
_database_code_amcsd             0008368
_diffrn_ambient_pressure         2.65e+06
_cell_formula_units_Z            4
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    3.640
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006786
Effect of pressure on the thermal expansion of MgO up to 8.2 GPa Sample: Run1 at T = 373 K, P = 2.68 GPa
Zhang, J.; Physics and Chemistry of Minerals 27 (2000) 145–148; doi:10.1007/s002690050001

data_9006787
_publ_section_title
;
 Effect of pressure on the thermal expansion of MgO up to 8.2 GPa
 Sample: Run1 at T = 373 K, P = 2.68 GPa
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              145
_journal_page_last               148
_journal_paper_doi               10.1007/s002690050001
_journal_volume                  27
_journal_year                    2000
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.1942
_cell_length_b                   4.1942
_cell_length_c                   4.1942
_cell_volume                     73.781
_database_code_amcsd             0008369
_diffrn_ambient_pressure         2.68e+06
_cell_formula_units_Z            4
_diffrn_ambient_temperature      373
_exptl_crystal_density_diffrn    3.628
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006787
Effect of pressure on the thermal expansion of MgO up to 8.2 GPa Sample: Run1 at T = 473 K, P = 2.62 GPa
Zhang, J.; Physics and Chemistry of Minerals 27 (2000) 145–148; doi:10.1007/s002690050001

data_9006788
_publ_section_title
;
 Effect of pressure on the thermal expansion of MgO up to 8.2 GPa
 Sample: Run1 at T = 473 K, P = 2.62 GPa
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              145
_journal_page_last               148
_journal_paper_doi               10.1007/s002690050001
_journal_volume                  27
_journal_year                    2000
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.1988
_cell_length_b                   4.1988
_cell_length_c                   4.1988
_cell_volume                     74.025
_database_code_amcsd             0008370
_diffrn_ambient_pressure         2.62e+06
_cell_formula_units_Z            4
_diffrn_ambient_temperature      473
_exptl_crystal_density_diffrn    3.616
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006788
Effect of pressure on the thermal expansion of MgO up to 8.2 GPa Sample: Run1 at T = 573 K, P = 2.66 GPa
Zhang, J.; Physics and Chemistry of Minerals 27 (2000) 145–148; doi:10.1007/s002690050001

data_9006789
_publ_section_title
;
 Effect of pressure on the thermal expansion of MgO up to 8.2 GPa
 Sample: Run1 at T = 573 K, P = 2.66 GPa
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              145
_journal_page_last               148
_journal_paper_doi               10.1007/s002690050001
_journal_volume                  27
_journal_year                    2000
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.2039
_cell_length_b                   4.2039
_cell_length_c                   4.2039
_cell_volume                     74.295
_database_code_amcsd             0008371
_diffrn_ambient_pressure         2.66e+06
_cell_formula_units_Z            4
_diffrn_ambient_temperature      573
_exptl_crystal_density_diffrn    3.603
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006789
Effect of pressure on the thermal expansion of MgO up to 8.2 GPa Sample: Run1 at T = 673 K, P = 2.66 GPa
Zhang, J.; Physics and Chemistry of Minerals 27 (2000) 145–148; doi:10.1007/s002690050001

data_9006790
_publ_section_title
;
 Effect of pressure on the thermal expansion of MgO up to 8.2 GPa
 Sample: Run1 at T = 673 K, P = 2.66 GPa
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              145
_journal_page_last               148
_journal_paper_doi               10.1007/s002690050001
_journal_volume                  27
_journal_year                    2000
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.2081
_cell_length_b                   4.2081
_cell_length_c                   4.2081
_cell_volume                     74.517
_database_code_amcsd             0008372
_diffrn_ambient_pressure         2.66e+06
_cell_formula_units_Z            4
_diffrn_ambient_temperature      673
_exptl_crystal_density_diffrn    3.593
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006790
Effect of pressure on the thermal expansion of MgO up to 8.2 GPa Sample: Run1 at T = 773 K, P = 2.61 GPa
Zhang, J.; Physics and Chemistry of Minerals 27 (2000) 145–148; doi:10.1007/s002690050001

data_9006791
_publ_section_title
;
 Effect of pressure on the thermal expansion of MgO up to 8.2 GPa
 Sample: Run1 at T = 773 K, P = 2.61 GPa
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              145
_journal_page_last               148
_journal_paper_doi               10.1007/s002690050001
_journal_volume                  27
_journal_year                    2000
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.2143
_cell_length_b                   4.2143
_cell_length_c                   4.2143
_cell_volume                     74.847
_database_code_amcsd             0008373
_diffrn_ambient_pressure         2.61e+06
_cell_formula_units_Z            4
_diffrn_ambient_temperature      773
_exptl_crystal_density_diffrn    3.577
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006791
Effect of pressure on the thermal expansion of MgO up to 8.2 GPa Sample: Run1 at T = 873 K, P = 2.64 GPa
Zhang, J.; Physics and Chemistry of Minerals 27 (2000) 145–148; doi:10.1007/s002690050001

data_9006792
_publ_section_title
;
 Effect of pressure on the thermal expansion of MgO up to 8.2 GPa
 Sample: Run1 at T = 873 K, P = 2.64 GPa
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              145
_journal_page_last               148
_journal_paper_doi               10.1007/s002690050001
_journal_volume                  27
_journal_year                    2000
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.2202
_cell_length_b                   4.2202
_cell_length_c                   4.2202
_cell_volume                     75.162
_database_code_amcsd             0008374
_diffrn_ambient_pressure         2.64e+06
_cell_formula_units_Z            4
_diffrn_ambient_temperature      873
_exptl_crystal_density_diffrn    3.562
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006792